Accepted Manuscript Simultaneous removal of polycyclic aromatic hydrocarbons and heavy metals from water using granular activated carbon Dinushika Eeshwarasinghe, Paripurnanda Loganathan, Saravanamuthu Vigneswaran PII:
To appear in:
Received Date: 11 December 2018 Revised Date:
5 February 2019
Accepted Date: 7 February 2019
Please cite this article as: Eeshwarasinghe, D., Loganathan, P., Vigneswaran, S., Simultaneous removal of polycyclic aromatic hydrocarbons and heavy metals from water using granular activated carbon, Chemosphere (2019), doi: https://doi.org/10.1016/j.chemosphere.2019.02.033. This is a PDF file of an unedited manuscript that has been accepted for publication. As a service to our customers we are providing this early version of the manuscript. The manuscript will undergo copyediting, typesetting, and review of the resulting proof before it is published in its final form. Please note that during the production process errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain.
ACCEPTED MANUSCRIPT 1
Declaration of interest: None
Simultaneous removal of polycyclic aromatic hydrocarbons and heavy
metals from water using granular activated carbon
Dinushika Eeshwarasinghe, Paripurnanda Loganathan, Saravanamuthu Vigneswaran*
Faculty of Engineering, University of Technology Sydney (UTS), P.O. Box 123, Broadway,
NSW 2007, Australia
*Corresponding author. Tel.:+61 2 95142641, fax: +61 2 95142633. Email: [email protected]
M AN U
Polycyclic aromatic hydrocarbons (PAHs) and heavy metals are dangerous pollutants that
commonly co-occur in water. An adsorption study conducted on the simultaneous removal of
PAHs (acenaphthylene, phenanthrene) and heavy metals (Cd, Cu, Zn) by granular activated
carbon (GAC) showed that, when these pollutants are present together, their adsorption was
less than when they were present individually. The adsorptive removal percentage of PAHs
(initial concentration 1 mg/L) was much higher than that of heavy metals (initial
concentration (20 mg/L). The reduction in adsorption of PAHs by heavy metals followed the
heavy metals’ adsorption capacity and reduction in the negative zeta potential of GAC order
ACCEPTED MANUSCRIPT (Cu > Zn > Cd). In contrast, PAHs had little effect on the zeta potential of GAC. The
Langmuir adsorption capacities of acenaphthylene (0.31-2.63 mg/g) and phenanthrene (0.74-
7.36 mg/g) on GAC decreased with increased metals’ concentration with the reduction
following the order of the metals’ adsorption capacity. The kinetic adsorption data fitted to
Weber and Morris plots, indicating intra-particle diffusion of both PAHs and heavy metals
into the mesopores and micropores in GAC with the diffusion rates. This depended on the
type of PAH and metal and whether the pollutants were present alone or together.
Keywords: heavy metals, polycyclic aromatic hydrocarbon, adsorption, zeta potential, water
M AN U
Elevated concentrations of heavy metals and polycyclic aromatic hydrocarbons
(PAHs) are known to have adverse effects on the aquatic environment due to their high
toxicity and long persistence. They can be potentially carcinogenic, mutagenic or allergenic
to humans and furthermore produce many other toxicity outcomes when they enter via the
aquatic food chain [1-6]. They are very commonly found to occur together and their
combined toxicity is reported to be higher than their individual toxicities .
Several treatment methods have been used to remove these pollutants from water such
as ion exchange /adsorption, biodegradation, photocatalysis oxidation, chemical precipitation,
membrane filtration, and electrochemical techniques [1,4,5,8-11]. Of these, adsorption is the
most cost-effective, simple, flexible and efficient process. As well, it produces minimum
chemical or biological sludge and the adsorbent can be regenerated and reused which leads to
a more cost-effective process. 2
ACCEPTED MANUSCRIPT Numerous studies have been reported on the adsorptive removal of heavy metals
[1,8,9] and PAHs [10-13] but very few of these have dealt with the simultaneous removal of
both of these pollutants. Simultaneous removal is important because PAHs’ and heavy
metals’ co-occurrence is very common in the environment, especially when the water
contains both industrial and domestic waste discharges  and in stormwaters containing
road-deposited sediments [15,16]. Considering the importance of the simultaneous removal
of these pollutants, in recent times more focus has been directed on conducting research on
Studies have reported both competitive and synergistic effects on the adsorption of
PAHs and heavy metals. Chen et al.  found that the presence of Cu decreased the
adsorption of naphthalene by wood black carbon and explained this outcome as due to
surface complexation of Cu to form hydration shells of dense water that competed with
naphthalene for adsorption. They also stated that pore blockage by the hydrated Cu inhibited
naphthalene adsorption. Huang et al.  compared the individual and combined adsorption
capacities of Cd and acenaphthene on a maghemite/mesoporous silica composite. They found
that the adsorption capacities decreased from those of individual capacities when
acenaphthene and Cd were present together. The competitive effect had a higher impact on
Cd adsorption than on acenaphthene adsorption. Also, Huang et al.  explained this as due
to faster adsorption of acenaphthene which allowed it to occupy the adsorption sites first
rather than Cd. In a study on the adsorption of Pb and pyrene in a soil, Pb curtailed the
adsorption of pyrene and pyrene reduced the adsorption of Pb due to competitive adsorption
M AN U
In contrast to the competitive effects, synergistic effects of heavy metals and PAHs
have also been reported in some studies. For example, Zhang et al.  found that Cu and
pyrene adsorption capacities on Fe functionalised mesoporous silica were higher when they
ACCEPTED MANUSCRIPT were present together than when they were present alone. They explained this observation as
due to the formation of a Cu-pyrene complex through cation-π interaction (non-covalent
binding force between metals and aromatic organic compounds) where the complex had
stronger affinity to the adsorbent than the individual components. Formation of pyrene-Cu
bridging was also suggested for the mutual promotion of the adsorption. The higher
adsorption of PAHs (acenaphthene, fluorene and fluoranthene) and heavy metals (Ni, Pb, Zn)
when they are present together compared to their individual presence was also reported for
adsorption on clay minerals . This was explained as due to the formation of a cation-π
bond with the effect being greater for the higher molecular weight PAHs. The reason for this
was the larger number of benzene rings providing more electrons for π-interaction. Tao et al.
[14,22] studied the effects of various metals on the adsorption of selected PAHs by aquatic
dead phytoplankton biomass and reported that a change in the concentration of the metals had
different effects on the adsorption behaviour of the PAHs. Sorption enhancement which
occurred at medium metal concentrations, was reportedly caused by these cation- π
interactions, and increased with the order of softness of the metals, and the π-donor strength
of the PAHs.
M AN U
Simultaneous adsorption of PAHs and heavy metals has not been studied in detail on
activated carbon (AC) adsorbent, which is one of the most popular and reliable adsorbents
used for removing both heavy metals [14,23-25] and PAHs [11-13,26]. Inner-sphere
complexation of heavy metals adsorption on AC has been established in previous studies
using zeta potential data  and this might have relevance to the simultaneous adsorption of
PAHs and heavy metals on AC. We have also shown earlier that the porosity of granular AC
(GAC) did influence PAH adsorption kinetics , which could in turn have an impact on the
mutual adsorption of PAH and heavy metals. These aspects will be used to explain the
simultaneous adsorption of heavy metals having different affinities to GAC and PAHs in the
ACCEPTED MANUSCRIPT 96
study presented here. The aims of the study, therefore, were to: firstly, determine the effects
of different concentrations of Cu, Cd, and Zn on the equilibrium and kinetics of
acenaphthylene and phenanthrene adsorption on GAC; secondly, determine the effect of
these two PAHs on the equilibrium and kinetics of adsorption of the three heavy metals; thirdly, explain the mechanism of adsorption using zeta potential data; and fourthly, model
the adsorption behaviour of the heavy metals and PAHs when they occur separately and
together. Such modelling has not been previously reported for simultaneous adsorption of
PAHs and heavy metals.
Materials and methods
M AN U
GAC (0.3–2.4 mm) for this study was purchased from James Cummins P/L, Australia. A particle size range of 400-800 µm was separated from the original material and used in the
experiments. The BET surface area, pore volume and average pore diameter of the GAC were
1010 m2/g, 0.69 cm3/g and 2.7 nm, respectively . The scanning electron micrographs of
the GAC (Fig. 1) revealed the presence of large numbers of micropores and mesopores which
may have resulted in GAC having high surface area.
Fig. 1. Scanning electron micrographs of GAC .
The PAHs used in the study were acenaphthylene (C12H8, logKow 3.94, molar volume
M AN U
168 cm3/mol) and phenanthrene (C14H10, logKow 4.46, molar volume 199 cm3/mol) . As
the PAHs were only partially soluble in water, their solutions were prepared from
concentrated stock solutions of each PAH dissolved in acetonitrile. The stock solutions
contained 20 mg PAH in 20 mL acetonitrile (1 g/L). Solutions employed for the studies were
prepared by diluting the stock solutions in 1% acetonitrile in Milli-Q® water. Acetonitrile and
PAHs used were spectroscopic grade materials purchased from Sigma-Aldrich, USA. Heavy
metals studied were Cu, Cd and Zn. Analytical grade (99% purity) nitrate salts of these
metals were employed in the experiments to prepare the heavy metals solution. These salts
were also purchased from Sigma-Aldrich (USA).
PAH concentration in the solution was determined using UV–VIS Spectrophotometry
(Shimadzu UV-1700). The absorbance values of acenaphthylene and phenanthrene were
determined at the wavelengths of 321 nm and 226 nm, respectively. These wavelengths
proved to be the optimum values for measuring the concentrations of these PAHs, both in the 6
ACCEPTED MANUSCRIPT presence and absence of heavy metals (Figs. S1, S3-S6, supplementary data). These PAHs’
concentrations were determined from standard curves of absorption vs concentrations of the
standards (Figs. S2, S7, S8). The glassware used in the experiments were initially washed and
rinsed with deionised water and then soaked overnight in dilute nitric acid bath before use.
PAH losses caused by photodegradation were minimised by covering all flasks containing
PAH solutions with aluminium foil. The flasks were also tightly sealed to prevent any losses
occurring through volatilisation. Heavy metal concentrations were determined using a
Microwave Plasma-Atomic Emission Spectrometer (Agilent 4100 MP-AES).
The zeta potential of GAC was conducted in the presence of 10-3 M of NaNO3 at pH
levels of 4, 5, and 6 with and without additions of heavy metals and PAHs using a Zetasizer
nano instrument (Nano ZS Zen3600, Malvern, UK). 10-3 M of NaNO3 was used to keep the
ionic strength of all solutions constant. The concentrations of GAC (< 0.075 mm particle
size), heavy metals, and PAHs in the suspensions were 0.6 g/L, 20 mg/L, and 1 mg/L,
respectively. The measurements were made after the suspensions were agitated in a flat
shaker at a speed of 120 rpm for 22 h. As the pH level changed from the initial pH during
PAHs and heavy metals adsorption, the pH levels were adjusted back to the initial pH after 3
h of shaking. pH adjustments were made by adding diluted HCl or NaOH. The initial pH, pH
after 3 h and the final pH were measured using a pH meter.
M AN U
A series of glass flasks containing 70 mL solutions at pH 5 in the presence of PAHs
and heavy metals together or individually were agitated with different GAC doses ranging
from 0.05 to 0.8 g/L in a flat shaker at 120 rpm for 5 h at room temperature (24 ± 1 °C). The 7
ACCEPTED MANUSCRIPT concentration of PAHs was 1 mg/L whereas that of heavy metals was 5, 20 or 50 mg/L.
Much higher concentrations were used for heavy metals to be in consistent with the
difference in concentrations between PAHs and heavy metals found in industrial and
domestic wastewaters where the concentrations of heavy metals are 10-1000 times those of
PAHs [6,27,28]. All solutions contained 0.005 M NaNO3 to ensure the ionic strength
remained constant. The suspensions were then filtered and subsequently the filtrates were
analysed for PAHs and heavy metals. The amount of PAH and heavy metal adsorption at
equilibrium, qe (mg/g), was calculated using the equation given below:
M AN U
where, C0 is initial concentration of PAH or heavy metal (mg/L), Ce is equilibrium
concentration of PAH or heavy metal (mg/L), V is volume of solution (L) and M is mass of
adsorbent (g). Percentage adsorption was calculated using the following equation and the data
were fitted to the mathematical models described in Table 1:
Percentage adsorption (%) =
The kinetics of adsorption was conducted at pH 5 in the presence of 0.005 M NaNO3
with an adsorbent dose of 0.3 g/L, PAHs concentration of 1 mg/L, and heavy metals
concentration of 20 mg/L, by shaking the suspensions at 120 rpm in a flat shaker at room
temperature. Samples were taken at different periods of time (10 min – 24 h), and after
filtration of the suspensions, the filtrates were analysed for PAHs and heavy metals. The
amount of PAH or heavy metal adsorption (qt) at time t was estimated as described below:
ACCEPTED MANUSCRIPT where, C0 is initial concentration of PAH or heavy metal (mg/L), Ct is concentration of PAH
or heavy metal at time t (mg/L), V is volume of the solution (L) and M is mass of adsorbent
(g). Both the equilibrium and kinetic adsorption data were fitted to the mathematical models
presented in Table 1.
M AN U
ACCEPTED MANUSCRIPT Table 1. Adsorption models used in the study Equation
Equilibrium models Langmuir1,2
qm KLCe 1 + KLCe Ce = equilibrium concentration of PAH or heavy metals (mg/L), q = amount of PAH adsorbed per unit mass of adsorbent (mg/g), qm = maximum amount of PAH or heavy metals adsorbed per unit mass of adsorbent (mg/g), KL = Langmuir constant (L/mg) relates the energy of adsorption qe =
qe = KfC e1 / n
M AN U
kf = Freundlich constant (mg/g) (L/mg)1/n, n = Freundlich constant, amount adsorbed per unit dosage of the adsorbent (mg/g) Dubinin– Radushkevich3,4
= the monolayer capacity, β = the activity coefficient related to mean adsorption energy and ɛ = Palanyi potential described as: where R = universal gas constant 8.314 (J/mol.K), the values
dqt = k1 (qe − qt ) dt qe = amount of PAH or heavy metals adsorbed at equilibrium (mg/g), qt = amount of PAH or heavy metals adsorbed at time t (h), (mg/g), k1 = rate constant for pseudo-first order adsorption (1/h)
Kinetic models Pseudo-first order 1,2
T = absolute temperature (K), From the plots of ln(qe) versus of β and qm were determined
Weber and Morris3,5
dqt 2 = k2 (qe − qt ) dt k2 = rate constant for pseudo-second order adsorption (g/mg.h)
qt = K p t 1 / 2 + B
kp = intra-particle diffusion rate constant (mg/(g.h1/2)), B = constant which provides a measure of the boundary layer thickness (mg/g) 1 Ahmanuzzaman ; 2 Kalaruban et al. ;]; 3Eeshwarasinghe et al. ; 4Alade et al. ; 5
Weber and Morris ,
185 186 10
ACCEPTED MANUSCRIPT 1873. Results and discussion 1883.1.
The adsorptive removals of PAHs in the presence and absence of heavy metals are shown as percentage removal of initially added PAHs for the initial PAHs concentration of 1
mg/L and heavy metals concentration of 20 mg/L in Fig. 2. For comparative purposes the
percentage of removal of heavy metals alone and in the presence of PAHs are also shown in
the same figure as well as in Fig. 3 where the results are illustrated more clearly by expanding
the Y-axis scale. Similar results are presented in Fig. S9 (supplementary data) for the initial
PAHs concentration of 1 mg/L and heavy metals concentration of 5 mg/L. The data show that
the percentages of PAHs removed are many times higher than those of the heavy metals
despite the latter having 20 times larger concentrations in solution. This indicates that PAHs
have higher affinity to GAC than heavy metals do. This is because the hydrophobic
interaction and H-bonding of the PAHs with the hydrophobic GAC surface and functional
groups [12,17] are more dominant than the cationic heavy metal ions’
exchange/chelation/complexation ability with the limited negatively charged functional
groups on GAC [17,24,31]. The removal percentages fell when PAH and heavy metals were
present together compared to their respective individual presence (Fig. 2 and 3), indicating
there was competition for adsorption between PAHs and heavy metals. The competitive
effect of PAHs on heavy metals adsorption is higher than the heavy metals’ effect on PAHs
adsorption. Enhancement of PAHs adsorption by heavy metals presence reported for other
adsorbents due to metal cation - π interaction [20,22] seems to be less important than the
competitive adsorption effect in the case of GAC.
M AN U
Because the percentage removal of PAHs and heavy metals presented in Fig. 2, 4 and
S9 depend on their initial concentrations the results are also presented as amounts adsorbed
(amounts removed) in Fig. 3, 5, S10 and S11. These figures show that in the case of 20 mg/L
ACCEPTED MANUSCRIPT of heavy metals the amounts of metals adsorbed are nearly twice those of acenaphthylene,
because the heavy metals concentrations were 20 times that of acenaphthylene. For
phenanthrene which has a higher affinity to GAC, the amounts adsorbed were nearly the
same as the heavy metals. However, when the heavy metals concentrations were reduced to 5
mg/L the amounts adsorbed for both the PAHs were higher than those of heavy metals,
indicating that the PAHs have higher affinity than heavy metals towards GAC.
At all GAC doses the adsorptive removal of phenanthrene was higher than that of acenaphthylene, both in the presence and absence of metals. This is probably due to the
higher hydrophobicity of the phenanthrene (log Kow 4.46; Kow 28,840) than that of
acenaphthylene (log Kow 3.94; Kow 8709), though pH changes during adsorption might have
also influenced the hydrophobicity difference between the two PAHs. This is consistent with
the findings of other studies which reported that the adsorption capacity of PAHs increased
with increasing log Kow [11-13]. Another reason could be the higher number of benzene rings
in phenanthrene (3 rings) compared to those in acenaphthylene (2 rings). Ge et al. 
reported that PAHs’ adsorption capacity increased when the number of benzene rings also
increased in PAH. This can be explained as being due to increased π-π complex formation
between the π-electrons of benzene rings and the active sites on an AC surface.
M AN U
Generally, the adsorption of PAHs was reduced by the metals in the order of Cu ≥ Zn
> Cd which is closely related to the metals’ adsorption capacity (Fig. 3). Sounthararajah et al.
 reported that the adsorption capacities of metals on GAC, both in batch and column
experiments, followed the order Cu > Zn > Cd. They explained this as due to Cu having the
lowest pK1 (first hydrolysis constant K1, highest tendency to form Cu(OH)+) and highest
hydroxide precipitate solubility product pKso (metal hydroxide precipitation potential high
when pKso is high) and Cd having the highest pK1 and lowest pKso. Erto et al.  also
reported similar explanations for the higher adsorption of Zn than Cd. They also stated that
ACCEPTED MANUSCRIPT Zn2+ being smaller in size than Cd2+ was able to penetrate smaller pores in AC and
furthermore it was less affected by steric hindrance during adsorption. McBride  provided
another explanation for the metal affinity order based on ionic potential (Z2/r) (Z is charge
and r is radius of the metal ion) which followed the same order as the affinity. The metals’
reaction with the functional groups can also influence the adsorption behaviour. The strength
of this reaction is reported to be higher for Cu than Zn .
M AN U
M AN U
Fig. 2. Percentage removal of acenaphthylene and phenanthrene compared with percentage
removal of heavy metals during their simultaneous adsorption on GAC in the presence of
0.005 M NaNO3 (PAH concentration 1 mg/L, metal concentration 20 mg/L).
253 254 14
M AN U
Fig. 3. Amount of acenaphthylene and phenanthrene removed compared with amount of
heavy metal removal during their simultaneous adsorption on GAC in the presence of 0.005
M NaNO3 (PAH concentration 1 mg/L, metal concentration 20 mg/L).
261 262 263
M AN U
Fig. 4. Percentage removal of heavy metals from solutions with and without the presence of
acenaphthylene and phenanthrene (solutions with initial concentrations: 0.005 M NaNO3,
PAH 1 mg/L, metal 20 mg/L). 16
M AN U
Fig. 5. Amount of heavy metals adsorbed from solutions with and without the presence of
acenaphthylene and phenanthrene (solutions with initial concentrations: 0.005 M NaNO3,
PAH 1 mg/L, metal 20 mg/L). 17
ACCEPTED MANUSCRIPT 2773.2.
Since the adsorption of heavy metals is governed by metals’ electrostatic interaction with the GAC surface, the zeta potential of GAC which reflects the surface charge, was
studied at various pH levels in the presence of heavy metals and PAHs. The negative zeta
potential of GAC in the absence of metals had the highest values (Fig. 6 and 7) which favours
the adsorption of the positively charged metals and it increased with pH due to increased
deprotonation of acidic functional groups. The data showed that the zero point of charge
(ZPC, pH at which the net charge is zero) of GAC was 4.2. The low zero point of charge
suggests that the GAC surface predominantly comprises -COOH functional groups .
The addition of PAHs to GAC suspensions had little effect on the zeta potential
because the PAHs had very few charges (Fig. 6 and 7). However, the addition of heavy
metals had strong effects on the zeta potential of GAC by drastically reducing the negative
surface potential. Addition of Cu reversed the negative zeta potential of GAC to positive
values at all pH values and Zn alone or with acenaphthylene either changed the negative
potential to zero or to positive values at pH values less than 5.5. The extent of reduction of
the negative zeta potential followed the same order of the adsorption capacity of the metals
(Cu > Zn > Cd) (Fig. 5). The strong reduction in the negative zeta potential indicates that the
metals were adsorbed by inner-sphere complexation (specific adsorption) by exchanging with
the protons on the GAC surface functional groups . The possible reasons for the
differences between the metals in alteration of the zeta potential were same as the metals’
adsorption capacity differences discussed in the earlier section.
M AN U
M AN U
Fig. 6. Effect of pH on the zeta potential of GAC (0.6 g/L) with and without metals (20
mg/L) and acenaphthylene (1 mg/L).
Fig. 7. Effect of pH on the zeta potential of GAC (0.6 g/L) with and without metals (20
mg/L) and phenanthrene (1 mg/L).
ACCEPTED MANUSCRIPT 3063.3.
pH changes during adsorption
At all initial pH levels, the pH increased for all treatments (∆pH positive) (Fig. 8). The ∆pH was highest for the lowest initial pH of 4 because, at this low pH, the protons (H+)
which are at high concentration in solution, adsorb onto the negatively charged sites on GAC.
This causes a decrease in their concentration in solution, thus producing a higher pH .
However, this increase in pH is lowered when heavy metals are added to the GAC because:
firstly, the metals compete with protons for adsorption; and secondly, protons are released to
the solution by exchanging with the metals adsorbed [29,37]. In the presence of PAHs, heavy
metals adsorption declined due to competition for adsorption with PAHs and therefore the
increase in pH remained approximately the same as in the GAC alone treatment except for
Cu which has higher adsorption capacity than the other metals even when PAHs are present.
Consistent with this data, the zeta potential of GAC was reversed from negative to positive
values in the presence of Cu and Cu + PAH (Fig. 6 and 7).
M AN U
As the initial pH increased, ∆pH was reduced because the adsorption of protons
declined due to the presence of lower proton concentration in solution and the higher
adsorption of metals releasing more protons [36,37]. This is more striking for Cu than Cd and
Zn because Cu was adsorbed in higher quantities.
M AN U
Fig. 8. Effect of initial pH, heavy metal, and PAH on change in pH (∆pH = final pH – initial
pH) during adsorption on GAC.
Fig. 9 shows that there is a negative relationship between ∆pH and ∆zeta potential
(zeta potential of GAC in the presence of heavy metals with and without PAHs – zeta
potential of GAC alone). As the initial pH increased from 4 to 6, ∆zeta potential increased
because specific adsorption (inner-sphere complexation) of metals, especially Cu and Zn,
increased . During the specific adsorption of metals, protons (H+) are released from the
functional groups on the GAC surface. The final pH was thus reduced and ∆pH decreased. At
the initial pHs of 5 and 6, ∆zeta potential followed the order Cu > Zn > Cd but ∆pH followed
the reverse order of Cd ≥ Zn > Cu, regardless of the presence or absence of PAHs.
340 341 342 343
Fig.9 Relationship between ∆pH (Final pH - initial pH) and ∆zeta potential (zeta potential of GAC with heavy metals and PAHs – zeta potential of GAC alone) at three initial pHs during adsorption ( - ∆zeta potential; , and - ∆pH)
M AN U
344 345 22
ACCEPTED MANUSCRIPT 3463.4.
Equilibrium adsorption modelling
Three adsorption models, namely Langmuir, Freundlich and Dubinin–Radushkevick models were used to describe the equilibrium adsorption data. Of these models, Langmuir model
satisfactorily described the data for both PAHs with and without metals at different
concentrations (Tables 3 and 4). The R2 values ranged from 0.60 to 0.88 for a degree of
freedom of data points of 8 (9 data points). This means that the model explained 60-88% of
the variation of data. R2 value > 0.76 (correlation coefficient, r = 0.87) for a degree of
freedom of 8 indicates a very highly significant relationship . R2 value > 0.59 (r = 0.76)
indicates a highly significant relationship. Freundlich model fitted well to the data for
phenanthrene (Table 4) except for phenanthrene with 50 mg/L concentration of metals. But it
failed to satisfactorily describe the data for acenaphthylene. Dubinin–Radushkevick model
satisfactorily described the data for both PAHs in the absence of metals but the data fit to this model
was poor in the presence of metals at most of the concentrations.
M AN U
The fairly satisfactory data fit to Langmuir model may indicate that the PAHs were
adsorbed as monolayers on the GAC. The Langmuir maximum adsorption capacity of
phenanthrene (7.36 mg/g) was higher than that of acenaphthylene (2.63 mg/g) due to the
higher hydrophobicity of the former (log Kow 4.46) than the latter (log Kow 3.94). The
presence of metals decreased the adsorption capacity with this effect becoming stronger as
the metal concentration increased because of competitive adsorption. The decrease in
adsorption capacity reached its highest point in the presence of Cu and its lowest when Cd
was present for reasons explained earlier. From the Langmuir model parameter KL, another
parameter RL can be calculated by using the formula RL = 1 / (1+CmKL) (where Cm is the
maximum initial concentration of sorbate) to assess whether the adsorption process is
favourable or not. The calculated RL values for the two PAHs in the presence of all
ACCEPTED MANUSCRIPT 370
concentrations of heavy metals were in the range of 0.05 - 0.26. As these values are between
0 and 1, the adsorption process can be considered a favourable one .
Unlike PAHs adsorption, the adsorption of heavy metals alone or in the presence of PAHs did not fit to either of the two adsorption models. This is because the percentage
removal of these metals was low at the low GAC doses used in the study and the intense
competition of PAHs with heavy metals for adsorption.
M AN U
Dubinin–Radushkevick model R2
M AN U
Table 3. Model parameters for the adsorption of acenaphthylene on GAC at three metals concentrations in the presence of 0.005 M NaNO3.
Table 4. Model parameters for the adsorption of phenanthrene on GAC at three metals concentrations in the presence of 0.005 M NaNO3. Langmuir model
M AN U
ACCEPTED MANUSCRIPT 3833.5. Kinetic adsorption modelling 384
The pseudo-first order model fitted better to the adsorption kinetic data of PAHs in the presence of heavy metals compared to the pseudo-second order model (Table S1).
Conversely, the opposite trend occurred for the adsorption of heavy metals in the presence of
PAHs (Table S2). This indicates that PAHs are adsorbed generally by physical interaction
with GAC through hydrophobic interaction and van der Waals forces whereas heavy metals
are adsorbed chemically through exchange with protons in the functional groups on GAC.
These results are consistent with the zeta potential findings where heavy metals adsorption
markedly decreased the negative charges on GAC and even Cu reversed them into positive
charges (Figs. 6 and 7). In comparison, PAHs adsorption had only little effect on the zeta
potential of GAC.
M AN U
Because the GAC has numerous pores and channels, the kinetics of adsorption would have been influenced by PAHs’ and metals’ diffusion rates into these pores and channels.
This was investigated by fitting the data to the Weber and Morris model . The fit of the
data showed two distinct sets of straight lines with high R2 values (0.89-0.99) (Figs. 10 and
11, Table 5). The straight-line relationships’ and the initial line going through the origin in
the graph show that the rate of adsorption is controlled by intra-particle diffusion. The
straight-line plots indicate that initially the rate of adsorption was fast (high Ks1) followed by
a slower rate of adsorption (low Ks2) (Table 5). The faster rate of adsorption was probably
due to intra-particle diffusion into the mesopores and the slower rate was into the micropores.
Haro et al.  reported three straight lines when the data for the adsorption of acenaphthene
and fluorene on activated carbon were plotted according to Weber and Morris model. They
attributed the first line up to 10 min to external mass transfer and the other two from 10 min
to 4 h to intra-particle diffusion similar to our interpretation. The allocation of the data to the
two straight lines is arbitrary by eye-estimate using the limited data which is clear for PAHs
ACCEPTED MANUSCRIPT 408
but not so much for the metals. Therefore, more data are required especially at longer times in
future studies to confirm the above explanations.
The diffusion rate into the mesopores (Ks1) was faster for acynaphthylene (molar volume 168 cm3/mol) than that for phenanthrene (molar volume 199 cm3/mol) irrespective of
the type of metals present because of its smaller size. However, this pattern was not noticed
in the rate of diffusion into the micropores (Ks2). With reference to the metals, generally, no
difference in the rate of diffusion into the mesopores was observed, but in the micropores the
heavy metals’ rate of diffusion was higher than that of PAHs.
M AN U
416 417 418
EP AC C
Fig. 10. Weber and Morris plots of (A) rate of adsorption of phenanthrene in the presence of
heavy metals; (B) rate of adsorption of acynaphthylene in the presence of heavy metals (PAH
1 mg/L, metals 20 mg/L, GAC dose 0.3 g/L).
M AN U
Fig. 11. Weber and Morris plots of (A) rate of adsorption of metals in the presence of
phenanthrene; (B) rate of adsorption of metals in the presence of acynaphthylene (1 mg/L)
(PAH 1 mg/L, metals 20 mg/L, GAC dose 0.3 g/L).
ACCEPTED MANUSCRIPT 433
Table 5. Weber-Morris plot parameters for the adsorption of PAHs and heavy metals in the
presence of each other Weber-Morris long-term
M AN U
4374. Conclusions 438
In solutions containing both PAHs (acenaphthylene or phenanthrene) and heavy
metals (Cd, Cu or Zn) the adsorptive removal of PAHs using GAC was greater than those of
heavy metals, even with the latter at 20 times higher concentration. The adsorptive capacities 30
ACCEPTED MANUSCRIPT of both PAHs and heavy metals were reduced in the presence of both compared to their
capacities when they were present separately. This was due to competition for adsorption,
despite their adsorption mechanisms being different. Copper and Zn reduced the adsorption
of PAHs more than Cd did. Similarly, PAHs reduced the adsorption of Cd more than the
other metals. These results were explained using zeta potential data where Cu and Zn reduced
the negative charges on the GAC more than Cd did – the negative charges were even reversed
to positive values in the presence of Cu. The adsorption capacity was higher for phenanthrene
than for acenaphthylene, which was consistent with the higher hydrophobicity of
phenanthrene. The Langmuir adsorption capacity for both the PAHs decreased with increased
concentration of metals, the effect being in the order Cu > Zn > Cd. The kinetic adsorption
data fitted to the Weber and Morris plots indicating intra-particle diffusion of both PAHs and
heavy metals into the mesopores and micropores in GAC. The diffusion rate was higher in all
cases in the mesopores which occurred when the adsorption process began. The rate of
diffusion into mesopores was faster for acenaphthylene than phenanthrene irrespective of the
type of metal present, consistent with their size difference. The rate of diffusion in both
mesopores and micropores was in the order Cu > Zn > Cd in the presence of either of the
M AN U
This study was financially supported by the Cooperative Research Centre for Contamination
Assessment and Remediation of the Environment (CRC CARE) (project number
463 464 465
ACCEPTED MANUSCRIPT 466
 M. Ahmaruzzaman, Industrial wastes as low-cost potential adsorbents for the treatment
of wastewater laden with heavy metals, Adv. Colloid Interface Sci. 166 (2011) 36-59.  H.I. Abdel-Shafy, M.S.M. Mansour, A review on polycyclic aromatic hydrocarbons: Source, environmental impact, effect on human health and remediation, Egyptian J.
Petroleum 25 (2016) 107-123.
 B. Armstrong, E. Hutchinson, J. Unwin, T. Fletcher, Lung cancer risk after exposure to
polycyclic aromatic hydrocarbons: a review and meta-analysis, Environ. Health Perspect.
112 (2004) 970-978.
478 479 480 481
M AN U
Manage. 92 (2011) 407-418.
 A.K. Haritash, C.P. Kaushik, Biodegradation aspects of polycyclic aromatic hydrocarbons (PAHs): a review, J. Hazard. Mater. 169 (2009) 1-15.
 F. Fu, Q Wang, Removal of heavy metal ions from wastewater: A review, J. Environ.
 A.T. Lawal, Polycyclic aromatic hydrocarbons: A review, Cogent Environ. Sci. 3 (2017) 1339841, 89 pages.
 P.T. Gauthier, W.P. Norwood, E.E. Prepas, G.G. Pyle, Metal-PAH mixtures in the
aquatic environment: a review of co-toxic mechanisms leading to more-than-additive
outcomes, Aquat. Toxicol. 154 (2014) 253–269.
484 485 486
 S.E. Baily, T.J. Olin, R.M. Bricka, D.D. Adrian, A review of potentially low-cost sorbents for heavy metals, Water Res. 33 (199) 2469-2479.  M. Hua, S. Zhang, B. Pan, W. Zhang, L. Lv, Q. Zhang, Heavy metal removal from
water/wastewater by nanosize metal oxides: A review, J. Hazard. Mater. 211-212 (2012)
ACCEPTED MANUSCRIPT 489 490
 S. Lamichhane, K.C. Balkrishna, R. Sarukkalige, Polycyclic aromatic hydrocarbons (PAHs) removal by sorption: A review, Chemosphere 148 (2016) 336-353.  S.M. Yakout, A.A. Daifullah, S.A. El-Reefy, Adsorption of naphthalene, phenanthrene
and pyrene from aqueous solution using low-cost activated carbon derived from
agricultural wastes, Adsorpt. Sci. Technol. 31 (2013) 293-302.
 D. Eeshwarasinghe, P. Loganathan, M. Kalaruban, D.P. Sounthararajah, J. Kandasamy,
S. Vigneswaran, Removing polycyclic aromatic hydrocarbons from water using granular
activated carbon: kinetic and equilibrium adsorption studies, Environ. Sci. Pollut. Res. 25
M AN U
 C. Valderrama, X. Gamisans, J.L. Cortina, A. Farrán, F.X. De las Heras, Evaluation of polyaromatic hydrocarbon removal from aqueous solutions using activated carbon and
hyper‐crosslinked polymer (Macronet MN200), J. Chem. Technol. Biotechnol. 84
 Y. Tao, W. Li, B. Xue, J. Zhong, S. Yao, Q. Wu, Different effects of copper (II),
cadmium (II), and phosphate on the sorption of phenanthrene on the biomass of
cyanobacteria, J. Hazard. Mater. 261 (2013) 21-28.  P. Loganathan, S. Vigneswaran, J. Kandasamy, Road-deposited sediments pollutants: a
critical review of their characteristics, source apportionment, and management, Crit. Rev.
Environ. Sci. Technol.43 (2013) 1315-1348.
 T.C. Nguyen, Pollutants in road-deposited sediments: characteristics, mobility,
bioavailability and remediation. Ph D thesis submitted to University of Technology
Sydney, Australia (2006).
 J. Chen, D. Zhu, C. Sun, Effect of heavy metals on the sorption of hydrophobic organic compounds to wood charcoal, Environ. Sci. Technol. 41 (2007) 2536-2541. 33
ACCEPTED MANUSCRIPT 513
 Y. Huang, A.N. Fulton, A.A. Keller, Simultaneous removal of PAHs and metal
contaminants from water using magnetic nanoparticle adsorbents, Sci. Total Environ. 571
 J. Aissaoui, M. Kacem, P. Dubujet, A. Mgaidi, Study of multi compound sorption of lead and pyrene on a reconstituted soil: batch and fixed bed column tests, Soil Sediment
Contam. 26 (20170 404-425.
 Z. Zhang, X. Hou, X. Zhang, H. Li, The synergistic adsorption of pyrene and copper
onto Fe(III)functionalized mesoporous silica from aqueous solution, Colloids and
Surfaces A: Physicochem. Eng. Aspects 520 (2017) 39-45.
M AN U
 M. Saeedi, L.Y. Li, J.R. Grace, Effect of organic matter and selected heavy metals on
sorption of acenaphthene, fluorene and fluoranthene onto various clays and clay
minerals. Environ. Earth Sci. 77 (2018) 305.
 Y. Tao, B. Xue, Z. Yang, S. Yao, S. Li, Effects of heavy metals on the sorption of
polycyclic aromatic hydrocarbons by Microcystis aeruginosa. J. Environ. Qual. 43
 T.A. Kurniawan, G.Y.S. Chan, W. Lo, S. Babel, Comparisons of low-cost adsorbents for
treating wastewaters laden with heavy metals, Sci. Total Environ. 366 (2006) 409-426.
 P. Loganathan, W.G. Shim, D.P. Sounthararajah, M. Kalaruban, T. Nur, S. Vigneswaran,
Modelling equilibrium adsorption of single, binary, and ternary combinations of Cu, Pb,
and Zn onto granular activated carbon, Environ. Sci. Pollut. Res. 25 (2018) 16664-16675.
 D.P. Sounthararajah, P. Loganathan, J. Kandasamy, S. Vigneswaran, Column studies on
the removal of dissolved organic carbon, turbidity and heavy metals from stormwater
using granular activated carbon, Desalin. water Treat. 57 (2016) 5045-5055.
ACCEPTED MANUSCRIPT 536
 A.O. Alade, O.S. Amuda, A.O. Ibrahim, Isothermal studies of adsorption of
acenaphthene from aqueous solution onto activated carbon produced from rice (Oryza
sativa) husk, Environ. Sci. Technol. 46 (2012) 87-95.
 L.J. Westholm, E. Repo, M. Sillanpaa, Filter materials for metal removal from mine drainage – a review, Environ. Sci. Pollut. Res. 21 (2014) 9109-9128.
 M. Manjuladevi, O.M. Sri, Heavy metals removal from industrial wastewater by nano
adsorbent prepared from cucumis melopeel activated carbon, J. Nanomed. Res. 5 (2017)
00102, 4 pages.
 M. Kalaruban, P. Loganathan, W.G. Shim, J. Kandasamy, H.H. Ngo, S. Vigneswaran,
Enhanced removal of nitrate from water using amine-grafted agricultural wastes, Sci.
Total Environ. 565 (2016) 503-510.
 W.J. Weber, J.C. Morris, Kinetics of adsorption on carbon from solution, J. Sanit. Eng. Div. - ASCE 89 (1963) 31-59.
M AN U
 L. Dong, L. Hou, Z. Wang, P. Gu, G. Chen, R. Jiang, A new function of spent activated carbon in BAC process: Removing heavy metals by ion exchange mechanism, J. Hazard.
Mater. 359 (2018) 76-84.
 X. Ge, Z. Wu, Z. Wu, Y. Yan, G. Cravotto, B. Ye, Enhanced PAHs adsorption using
iron-modified coal-based activated carbon via microwave radiation, J. Taiwan Inst.
Chem. Eng. 64 (2016) 235-243.
 D.P. Sounthararajah, P. Loganathan, J. Kandasamy, S. Vigneswaran, Effects of humic
acid and suspended solids on the removal of heavy metals from water by adsorption onto
granular activated carbon, Inter. J. Environ. Res. Public Health 12 (2015) 10475-10489.
 A. Erto, F. Di Natale, D. Musmarra, A.Lancia, Modeling of single and competitive adsorption of cadmium and zinc onto activated carbon, Adsorption 21 (2015) 611-621. 35
561 562 563 564
 M.B. McBride, Reactions controlling heavy metal solubility in soil, Adv. Soil Sci. 10 (1989) 1–56.  K. Park, C. Lee, S. Ryu, X. Yang, Zeta-potentials of oxygen and nitrogen enriched activated carbons, Carbon Letters 8 (2007) 321-325.
 S.A. Dastgheib, D.A. Rockstraw, Pecan shell activated carbon: synthesis,
characterization, and application for the removal of copper from aqueous solution,
Carbon 39 92001) 1849-1855.
 T.M. Little, F.J. Hills, Agricultural Experimentation, Design and Analysis, John Willey and Sons, New York. (1978).
M AN U
 R. Rusmin, B. Sarkar, Y. Liu, S. McClure, R. Naidu, Structural evolution of chitosan–
palygorskite composites and removal of aqueous lead by composite beads, Appl. Surf.
Sci. 353 (2015) 363-375.
 M. Haro, B. Cabal, J.B. Parra, C.O. Ania, On the adsorption kinetics and equilibrium of
polyaromatic hydrocarbons from aqueous solution, Adsorp. Sci. Tech. 29 (2011) 467-
ACCEPTED MANUSCRIPT Highlights GAC adsorption of polycyclic aromatic hydrocarbon (PAH) higher than heavy metals.
PAHs’ adsorption capacities reduced by heavy metals in the order, Cu > Zn > Cd.
GAC’s negative zeta potential reduced by adsorption of heavy metals: Cu > Zn > Cd.
Intra-particle diffusion of heavy metals and PAHs into GAC’s meso and micro pores.
Langmuir adsorption capacity of phenanthrene (higher log Kow)) > acenaphthylene.
M AN U
M AN U
Novelty of this study is demonstration of the interactive adsorption behaviour of polycyclic aromatic hydrocarbons (PAHs) and heavy metals (HMs) on granular activated carbon. Such a study has not been previously reported for any activated carbon which is a common adsorbent used in water treatment operations. Using zeta potential data of granular activated carbon in the presence and absence of HMs and PAHs in explaining the adsorption data is another novelty of the paper.